BaGa(2)MQ(6) (M = Si, Ge; Q = S, Se): a new series of promising IR nonlinear optical materials.
Yin, Wenlong; Feng, Kai; He, Ran; Mei, Dajiang; Lin, Zheshuai; Yao, Jiyong; Wu, Yicheng; Dalton transactions (Cambridge, England : 2003) 41 (2012) 5653–5661; doi:10.1039/c2dt12493a

data_7018930
_publ_section_title
;
 BaGa(2)MQ(6) (M = Si, Ge; Q = S, Se): a new series of promising IR
 nonlinear optical materials.
;
_journal_issue                   18
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              5653
_journal_page_last               5661
_journal_paper_doi               10.1039/c2dt12493a
_journal_volume                  41
_journal_year                    2012
_chemical_formula_sum            'Ba Ga2 Ge Se6'
_chemical_formula_weight         823.13
_space_group_IT_number           146
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  'R 3'
_symmetry_space_group_name_H-M   'R 3 :H'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2011-11-05 # Formatted by publCIF
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   10.0075(14)
_cell_length_b                   10.0075(14)
_cell_length_c                   9.0903(18)
_cell_measurement_reflns_used    1185
_cell_measurement_temperature    93(2)
_cell_measurement_theta_max      30.9
_cell_measurement_theta_min      3.3
_cell_volume                     788.4(2)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      93(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Rigaku AFC10 diffractometer'
_diffrn_measurement_method       '\f and \w scan'
_diffrn_radiation_monochromator  'Graphite Monochromator'
_diffrn_radiation_source         'Rotating Anode'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0416
_diffrn_reflns_av_sigmaI/netI    0.0617
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            2532
_diffrn_reflns_theta_full        30.87
_diffrn_reflns_theta_max         30.87
_diffrn_reflns_theta_min         3.25
_exptl_absorpt_coefficient_mu    32.301
_exptl_absorpt_correction_T_max  0.126
_exptl_absorpt_correction_T_min  0.041
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'face indexed'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    5.201
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Block
_exptl_crystal_F_000             1062
_exptl_crystal_size_max          0.1540
_exptl_crystal_size_mid          0.1340
_exptl_crystal_size_min          0.0880
_refine_diff_density_max         1.848
_refine_diff_density_min         -1.295
_refine_diff_density_rms         0.266
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.00(3)
_refine_ls_extinction_coef       0.00282(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.846
_refine_ls_matrix_type           full
_refine_ls_number_parameters     33
_refine_ls_number_reflns         1117
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      0.846
_refine_ls_R_factor_all          0.0288
_refine_ls_R_factor_gt           0.0266
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0100P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0505
_refine_ls_wR_factor_ref         0.0509
_reflns_number_gt                1019
_reflns_number_total             1117
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2dt12493a.txt
_cod_data_source_block           BaGa2GeSe6
_cod_original_sg_symbol_H-M      R3
_cod_database_code               7018930